U.S. Department of Transportation
Federal Highway Administration
1200 New Jersey Avenue, SE
Washington, DC 20590
202-366-4000
Federal Highway Administration Research and Technology
Coordinating, Developing, and Delivering Highway Transportation Innovations
REPORT |
This report is an archived publication and may contain dated technical, contact, and link information |
Publication Number: FHWA-HRT-12-030 Date: August 2012 |
Publication Number:
FHWA-HRT-12-030
Date: August 2012 |
PDF Version (4.44 MB)
PDF files can be viewed with the Acrobat® Reader®
The flexural strength model 1 provides the best correlation between compressive strength and flexural strength with the LTPP data. The model form utilizes the power equation. This model will be most useful for cases when the compressive strength of the PCC has been determined through a routine cylinder break.
This model can be expressed as follows:
Where:
MR = Flexural strength, psi.
f'_{c,}= Compressive strength determined at the same age, psi.
The regression statistics for this model are presented in table 33. The model was developed using 185 data points, and the prediction has an R^{2} value of 45.2 percent and an RMSE value of 69 psi. Table 34 provides details of the range of data used to develop the model. The confidence limits are both within acceptable ranges for both the regressed coefficients (i.e., limits are positive numbers). Figure 173 and figure 174 show the predicted versus measured plot and the residual plot, respectively.
Parameter |
Estimate |
Standard Error |
Approximate 95 Percent Confidence Limits |
a |
22.7741 |
6.6362 |
9.6807 to 35.8674 |
b |
0.4082 |
0.0338 |
0.3416 to 0.4748 |
The model statistics for table 33 are as follows:
Parameter |
Minimum |
Maximum |
Average |
Compressive strength |
1,770 |
10,032 |
5,431 |
Flexural strength |
467 |
1,075 |
754 |
Figure 175 shows a comparison of the power models used to validate the data and also to develop a new correlation. Note that the three power models (the new equation developed for this study as well as the validation models) provide close estimates (within 50 psi) in the 4,500- to 5,500-psi compressive strength range.
The ACI and PCA models are plotted for comparison. Also plotted in figure 175 are the raw data that were used in the model. Clearly, the ACI equation is very conservative for this data. It also has been found to give a conservative estimate for several large datasets that have been used in flexural strength model prediction. Conversely, the PCA model fits the LTPP data more closely. The reasons for this lack of fit of the current data with the previous models may be too many to fully explain. The data used in models from prior studies often came from mixes batched under controlled laboratory experiments and were typical of paving and structural concrete. The mixes used in the current model developed from LTPP data relies on only mixes proportioned for typical paving operations. Furthermore, the LTPP data used are from many projects widely dispersed around the United States. This in itself makes the models more robust than any previous data used to make similar correlations.
The spread in the raw data about the prediction model in figure 175 indicates that there are factors other than compressive strength that influence the flexural strength of PCC. Among the various factors influencing flexural strength are the mix design parameters and age of the concrete. These variables were considered in the other models developed in this study.
Flexural strength model 2 provides a correlation between flexural strength and mix design parameters, specifically the unit weight and w/c ratio. Age is also a parameter in this model, which helps reduce some of the variability seen in the prediction relative to the predictions shown in figure 175. This model will be most useful for cases when the compressive strength of the PCC is not determined but mix design information is available. Also, the user has the option of predicting the 28-day strength value for design or estimating the strength at traffic opening time.
This model can be expressed as follows:
Where:
MR_{t} = Flexural strength at age t years, psi.
w/c = Water to cement ratio.
uw = Unit weight, lb/ft^{3}.
t = Pavement age, years.
The regression statistics for this model are presented in table 35. The model was developed using 62 data points, and the prediction has an R^{2} value of 61.1 percent and an RMSE value of 69 psi. Table 36 provides details of the range of data used to develop the model. Figure 177 and figure 178 show the predicted versus measured plot and the residual plot, respectively.
Variable |
DF |
Estimate |
Standard Error |
t-value |
P_{r} > t |
VIF |
Intercept |
1 |
676.0159 |
277.7887 |
2.43 |
0.0181 |
0 |
w/c |
1 |
-1,120.31 |
141.3573 |
-7.93 |
< 0.0001 |
1.00591 |
Unit weight |
1 |
4.1304 |
1.88934 |
2.19 |
0.0329 |
1.00311 |
Ln(age) |
1 |
35.74627 |
8.78516 |
4.07 |
0.0001 |
1.00619 |
The model statistics for table 35 are as follows:
Parameter |
Minimum |
Maximum |
Average |
w/c ratio |
0.27 |
0.58 |
0.40 |
Unit weight |
124 |
151 |
142 |
Pavement age |
0.0384 |
1.0000 |
0.3169 |
Flexural strength |
467 |
978 |
742 |
The data used in the previous model also provided a good correlation by replacing the w/c ratio parameter with CMC. The model is expressed as follows:
Where:
MR_{t} = Flexural strength at age t years, psi.
CMC = Cementitious materials content, lb/yd^{3}.
uw = Unit weight, lb/ft^{3}.
t = Pavement age, years.
The regression statistics for this model are presented in table 37. The model was developed using 62 data points, and the prediction has an R^{2} value of 70.2 percent and an RMSE value of 80 psi. Table 38 provides details of the range of data used to develop the model. Figure 180 and figure 181 show the predicted versus measured plot and the residual plot, respectively.
Figure 182 to figure 185 present the sensitivity of the mix design-based flexural strength models to CMC, w/c ratio, unit weight, and age. Figure 182 and figure 183 show that prediction models in figure 176 and figure 179 do not show any sensitivity to CMC and w/c ratio. For typical values of these parameters, the flexural strength prediction from these two models could show a difference of about 200 psi for extreme values of w/c ratios. However, within a typical range of 0.35 to 0.45, the flexural strength prediction is within 50 psi. Similar trends are evident for the w/c ratio parameter. Therefore, if all details about a mix design are available, it is highly recommended that both models be used to predict flexural strength so that the user has a fair estimate of the MR range. Figure 184 shows that the predictions are close from both models. Likewise, figure 185, which is more or less a flexural strength gain model for a typical mix design, shows close predictions from both models.
Variable |
DF |
Estimate |
Standard Error |
t-value |
P_{r} > t |
VIF |
Intercept |
1 |
24.15063 |
236.7606 |
0.1 |
0.9191 |
0 |
CMC |
1 |
0.55579 |
0.05563 |
9.99 |
< 0.0001 |
1.01522 |
Unit weight |
1 |
2.96376 |
1.66087 |
1.78 |
0.0796 |
1.01253 |
Ln(age) |
1 |
35.54463 |
7.68504 |
4.63 |
< 0.0001 |
1.00573 |
The model statistics for table 37 are as follows:
Parameter |
Minimum |
Maximum |
Average |
CMC |
388 |
936 |
668 |
Unit weight |
124 |
151 |
142 |
Pavement age |
0.0384 |
1.0000 |
0.3169 |
Flexural strength |
467 |
978 |
742 |